Open Access Treatment of Polyamides Fabrics with ... Treatment of Polyamides Fabrics with...
Embed Size (px)
Transcript of Open Access Treatment of Polyamides Fabrics with ... Treatment of Polyamides Fabrics with...
6 The Open Textile Journal, 2010 3, 6-13
1876-5203/10 2010 Bentham Open
Treatment of Polyamides Fabrics with Cyclodextrins to Improve Antimicrobial and Thermal Stability Properties
A. Bendak, O.G. Allam and L.K. El Gabry*
Textile Research Division, National Research Centre, Dokki, Cairo, Egypt
Abstract: Treatments of polyamide 6, Quiana and Nomex fabrics with - Cyclodextrin(CD) or monochlorotriazinyl -Cyclodextrin(CD-T) were investigated. Significant improvements in antimicrobial and thermal stability uniformity were observed. The colour values and fastness of the coloured fabrics to washing and perspiration were given. The untreated and treated fabrics were characterized by infrared spectroscopy (FTIR), differential thermal analysis (DTA) and thermogravimetric analysis (TGA). The changes in yellowness, moisture regain, roughness, tensile strength, elongation and antimicrobial activity have been studied. The TGA indicated that the temperature of burning Tb value lies at 471oC-472oC for CD treated polyamide 6 while it lies at 475oC-490oC for CD-T treated one. This may afford the use of CD-T in treatment of polyamide 6 to attain also some heat resistance than untreated one.
Keywords: Polyamide 6, Quiana, Nomex, Reactive dyes, - cyclodextrin, monochlorotriazinyl, Antimicrobial Infrared, DTA, TGA, and Tb.
1. INTRODUCTION Cyclodextrins are cyclic oligosaccharides. These molecu-les are able to form inclusion complexes with a large number of organic molecules. The properties of cyclodextrins enable them to be used in a variety of different textile applications. Owing to the complexing abilities of cyclodextrins, textiles with new functional properties could be made available . - Cyclodextrin (CD-T) was used as a low environmental impact additive in dyeing processes of polyamide fibres with azo disperses dyes . Efficient pretreatments of the textile fibres, temperature, pH and addition of electrolytes can influence the uniformity of their dyeing. Auxiliaries act with dye solution on the fibre interface or act as resolving of the dye molecules interface . The amount of remaining dyes in the waste water is significantly reduced when CD/dye complexes are formed . Cyclodextrins have a hydrophobic internal cavity so that they can improve the dye up take of azoic disperse dyes by polyester fibres . CD serves as a host in the formation of both soluble and solved crystalline inclusion complexes with large variety of non- covalently included guest molecules . Four- to 10-fold improvement of colour uniformity and minor changes of colour yield have been found upon dyeing Nylon 66 and microfiber Nylon 6 fabrics in the presence of cyclodextrin compared to dyeing without it. 1H NMR data supported the role of cyclodextrin as dye complexing agent. Product quality, however, was also dependent on fabric nature, since for conventional Nylon 6, color uniformity was not imp-
*Address correspondence to this author at the National Research Centre, Textile Research Division, Dokki, Cairo, Egypt; Tel: (202) 33335940; Fax: 33330931-3332242; E-mail: Lamiaa_gabry@yahoo.com
roved by the presence of cyclodextrin systems [7, 8]. Retarder/leveling effect of -cyclodextrin in dyeing process has been studied and the results were compared with that of a commercial product. In general, cyclodextrins were used in washing processes to remove the absorbed surfactants . -Cyclodextrin was tested as a dye complexing agent as a dye retardant in the dyeing of PAN fibres with cationic dyes. Significant improvement of colour uniformity and some improvements in colour depth were observed when PAN fibres were dyed in the presence of -cyclodextrin as compared to dyeing in the presence of a commercial retardant . The finishing process involved polymerization between citric acid and CDs, which yielded a cross-linked polymer that physically adhered to the surface of PA fibers. This permanent functionalization was characterized by evaluating the damping property with a polar liquid (glycerol) via the drop contact angle method for various rates of modification of the fabrics. The biological and microbiological effects of the PA, which were functionalized with hydroxypropylated derivate of -CD (HP--CDs) and charged with ciprofloxacin (CFX), were evaluated by cell culture assays . In the future cyclodextrins might play a significant role in the textile industry and might be used: (1) to remove surfact-ants from washed textiles; (2) to substitute surfactants; (3) in finishing textiles; (4) when bound chemically to fibers, to provide enhanced hydrophilicity and first of all, inclusion complex forming ability to immobilize perfumes, insect repellents, antimicrobial agents, etc . -cyclodextrin (CD)-based linear water-soluble polymers were synthesized. The synthesized water-soluble polymer was covalently fixed onto cotton surfaces by a polycon-densation reaction at controlled conditions. The grafting occurred through the formation of a crosslink between hydroxyl groups of cotton and CD polymer.This was confirmed using FTIR spectroscopy and DSC .
Treatment of Polyamides Fabrics with Cyclodextrins The Open Textile Journal, 2010, Volume 3 7
It is aimed in this investigation to carry out a systematic study on the pretreatment of polyamide 6, Nomex and Quiana fabrics with CD or CD T derivative to prepare antimicrobial polyamide fabrics. The effect of variation of the treatment conditions, such as concentration of CD and CD-T, and thermo fixation temperature is studied. The changes in the dyeing properties (colour value and fastness) of the treated polyamides fabrics are evaluated.
Knitted Polyamide 6 (aliphatic PA) was supplied from El-Shourbagy Co., Cairo, Egypt. Quiana (cyclic PA) and Nomex (aromatic PA) fibres were supplied by PCUK (Produits Chemiques Ugine Kuhlmann, Creil Cedex, France). The fabrics were scoured in aqueous bath for 30 minutes, at 60C using 2% nonionic detergent (o.w.f.) liquor ratio 1:50. The scoured fabrics were washed with warm water followed by rinsing for 5 minutes in cold water, and air dried.
-Cyclodextrin hydrate (CD), monochlortriazinyl -cyclodextrin Na-salt (CD-T) are products of Wacker Chemie GmbH, Munich, Germany. Quaternary ammonium salt (3-chloro-2-hydroxypropyl trimethylamonium chloride) was supplied from Floka (Germany).
The commercial dye samples. C.I. Reactive Red 84 (Ciba Specialty Chemicals), C.I. Reactive Blue 203 (Egypt Colours) and C.I. Reactive Yellow 1(Isama Dye. Egypt) were used.
The polyamides fabric were immersed in a solution con-taining 10-50 g/l (o. w .f) of -Cyclodextrin hydrate (CD), or monochlortriazinyl -cyclodextrin Na-salt (CD-T) which adjusted to pH 4 using acetic acid or citric acid at room temperature for 1h, then padded to pickup 100 %, dried at 80C for 10 min. and then fixed at 160C for 5 min. Finally the fabric is washed thoroughly with tap water and air dried. Also, polyamides fabrics were treated with solution con-taining 30g/l (o.w.f) of CD-T and 2g/l quaternary ammonium salt at the same conditions.
The dye bath was prepared by accurately weighing the dyestuff to give the prescribed shade. The dye was pasted with small amount of water and wetting agent. The paste was then dissolved by adding hot boiling water. The dye solution was then added to the dyeing bath, adjusted to pH 4.5 using acetic acid. The dye bath was heated to 80C, then added the sample to the dyeing bath and continued for 1 h. The dyed samples were then thoroughly washed in warm and cold water and air-dried.
2.4.1. Colour Value
Spectral reflectance measurements of the dyed fabrics were carried out using a recording filter Spectrophotometer Hunter lab (The Colour Management Company, USA). The colour value expressed as K/S of the dyed samples was determined by applying the Kubelka-Munk equation .
K / S =(1!R)2
Where R: is the decimal fraction of the reflectance of the dyed substrate. Ro: is the decimal fraction of the reflectance of the undyed substrate S: is the scattering coefficient K: is the absorption coefficient
2.4.2. Yellowness Index
Measurement of the yellowness index was carried out by using Hunter lab (The Colour Management Company, USA). Yellowness Index (YI) was determined using ASTM method E (313).
YI (E313) =100[1-(0.847 Z /Y)] Y, Z are the first numerical scale offered to quantify colour. YI: Yellowness Index of treated polyamide 6 sample.
2.4.3. Washing Fastness
The colour fastness to washing was determined according to the AATCC test method 611994 using a laundrometer. The soaped specimen (5x5cm) was sewed between two pieces of bleached wool and polyamide 6 in case of dyeing with reactive dyes. The composites were immersed into an aqueous solution containing 5 g/l soap and 2 g/l sodium carbonate, liquor ratio of 1:50 at 40C. The test was run for 40 minutes. The samples were then removed, rinsed twice in 100 ml of water at 40C for 15 minutes with occasional stirring and hand squeezing. This was followed by scouring in 100 ml of 0.014 % solution of acetic acid for one minute at 27C rinsing again for one minute in 100 ml water at 27C, followed by drying. Evaluation of the wash fastness was carried out using the Gray Scale reference for colour change .
2.4.4. Perspiration Fastness
0.25 g/l L-histidine monohydrochloride monohydrate. 10g/l of sodium chloride, 1g/l sodium hydrogen phosphate were dissolved in one litre of distilled water. Finally the pH was adjusted to 8 by sodium hydroxide solution